impact of sterilization by electron beam, gamma radiation ...kinampark.com/pl/files/cassan 2019,...
Embed Size (px)
Journal of Materials Science: Materials in Medicine (2019) 30:42https://doi.org/10.1007/s10856-019-6245-7
BIOMATERIALS SYNTHESIS AND CHARACTERIZATION
Impact of sterilization by electron beam, gamma radiation and X-rays on electrospun poly-(ε-caprolactone) fiber mats
Dominik de Cassan1 ● Anna Lena Hoheisel2,3 ● Birgit Glasmacher2,3 ● Henning Menzel 1
Received: 9 January 2019 / Accepted: 13 March 2019 / Published online: 27 March 2019© Springer Science+Business Media, LLC, part of Springer Nature 2019
AbstractBiodegradable polymers such as polycaprolactone (PCL) are increasingly used for electrospinning substrates for tissueengineering. These materials offer great advantages such as biocompatibility and good mechanical properties. However, inorder to be approved for human implantation they have to be sterilized. The impact of commonly used irradiationsterilization methods on electrospun PCL fiber mats was investigated systematically. Electron beam (β-irradiation), gammaand X-ray irradiation with two different doses (25 and 33 kGy) were investigated. To determine the impact on the fiber mats,mechanical, chemical, thermal properties and crystallinity were investigated. Irradiation resulted in a significant decrease inmolecular weight. At the same time, crystallinity of fiber mats increased significantly. However, the mechanical propertiesdid not change significantly upon irradiation, mostly likely because effects of a lower molecular weight were balanced withthe higher degree of crystallinity. The irradiation effects were dose dependent, a higher irradiation dose led to strongerchanges. Gamma irradiation seemed to be the least suited method, while electron beams (β irradiation) had a lower impact.Therefore, β irradiation is recommended as sterilization method for electrospun PCL fiber mats.
Pathogens on the surface or within a biomedical device cancause severe infections and can even lead to an explantationsurgery. Hence biomedical devices intended for humanimplantation require sterilization in order to fulfill reg-ulatory issues. These regulatory aspects, based on estab-lished standards, are set by organizations such as the USFood and Drug Administration or the Medical DeviceDirective for manufacturers within the EU [1, 2].
Several sterilization methods have been establishedover past decades. These methods include steam proces-sing/autoclaving , treatment with ethylene oxide ,plasma sterilization , as well as irradiation with
* Henning [email protected]
1 Institute for Technical Chemistry, Braunschweig University ofTechnology, Braunschweig, Germany
2 Institute for Multiphase Processes, Gottfried Wilhelm LeibnizUniversität Hannover, Hannover, Germany
3 Lower Saxony Centre for Biomedical Engineering, ImplantResearch and Development (NIFE), Hannover, Germany
Supplementary information The online version of this article (https://doi.org/10.1007/s10856-019-6245-7) contains supplementarymaterial, which is available to authorised users.
electron beams (beta irradiation) , gamma-radiation or X-rays . The sterilization method has to be chosenaccording to materials used for implants, because ster-ilization itself can be inappropriate, ineffective or evendestructive [8–11].
Electrospinning is a common technique for productionof structured scaffolds (fiber mats), which are similar toextracellular matrix (ECM) (for tissue-engineering appli-cations) [12–14]. These fiber mats are very versatile inapplication and for example used to produce wounddressings , nerve conduits , vascular grafts ,drug delivery systems  and implants for tendon/liga-ment-to-bone interfaces . In the laboratory, suchelectrospun scaffolds are typically sterilized using EtOHimmersion or UV irradiation. However, for use as animplantable biomedical device, these sterilization meth-ods are not approved by regulatory bodies [20, 21]. Theuse of electrospun scaffolds for biomedical devices istherefore not permissible using these simple sterilizationstrategies. On the other hand, it has been shown thatgamma irradiation can cause significant damage to elec-trospun polymeric scaffolds. In general high energyradiation like gamma-rays can lead to polymer chainscission and, depending on the polymer, result in lowermolecular weight or crosslinking [22, 23]. However, theseeffects do not necessarily lead to lower mechanical orbiological performance. Bosworth et al.  and Augus-tine et al.  produced various PCL scaffolds by dif-ferent electrospinning approaches and used gamma-radiation for sterilization. Bosworth et al. found in theirstudies that γ-irradiation lowers the molecular weight andultimate tensile stress of PCL fiber mats depending on theirradiation dose used . Augustine et al. found that alow irradiation dose first leads to improved mechanicalproperties but higher irradiation doses ultimately led to adecrease .
Due to relatively low melting temperature of PCL of60 °C some sterilization methods could damage thematerial or implant structure. Hence steam processing andautoclaving techniques are not applicable for PCL. Thisstudy therefore focusses on comparing the impact of threeestablished and approved low temperature sterilizationtechniques on electrospun PCL scaffolds: Electron beam(β), gamma radiation (γ) and X-rays. To investigate apossible dose dependent effect, two irradiation doses areused including the commonly used dose for medicaldevices sterilization of 25 kGy. While static tensile testingwas carried out to determine changes regarding materialsmechanical properties, size exclusion chromatography(SEC) was used to check for changes in molecular weightand differential scanning calorimetry (DSC) measure-ments to determine degree of crystallization and changesin thermal properties.
2 Materials and methods
Unless otherwise stated all chemicals used were purchasedfrom Sigma-Aldrich. PCL (Mn= 80,000) was also pur-chased from Sigma-Aldrich (Darmstadt, Germany). 2,2,2-Trifluoroethanol (TFE) was purchased from ABCR(Karlsruhe, Germany).
2.1 Electrospinning of PCL
A 17% (w/v) PCL in 2,2,2-trifluoroethanol (TFE) solutionwas loaded into a syringe connected by polyvinylchloride(PVC) tubing to a spinneret. A rotating aluminum drumcovered with polytetrafluoroethylene (PTFE) coated bakingpaper (ja!, REWE, Germany) was used as collector. Scaf-folds were produced with a voltage of 20 kV at a cir-cumferential speed of either 2 m/s for non-aligned butrandomly oriented fibers (r) or 8 m/s for aligned fibers (a).Spinneret to collector distance was set to 20 cm and thesolution flow rate to 3 ml/h. The electrospinning process ranfor 2 h.
Prior to sterilization specimens were cut into uniform stripsusing a rotary cutter (Dahle, Germany). Specimens had awidth of 10 mm and a free tensile test length of 40 mm inrotary direction. A set of unsterilized specimens served ascontrol. Sterilization was carried out by Mediscan (Sei-bersdorf, Austria). Each of the three irradiation types (β, γand X) was tested with two irradiation doses (25 and 33kGy).
2.3 Scaffold morphologies
Scaffolds were imaged with SEM (Hitachi S-3400N,Tokyo, Japan) to investigate alignment of fibers within twosample types of non-aligned and aligned fiber mats. SEMimages were analyzed with an image analysis software(AxioVision, Carl Zeiss, Jena, Germany).
2.4 Mechanical characterization
Static tensile testing was carried out using a universaltesting machine (5655, Instron, Norwood, USA). Speci-mens were mounted to the universal testing machine withpneumatic grips and tested with a crosshead speed of 40mm/min with a load cell of 500 N at 20 °C. Specimens werestretched until failure.
Thickness of specimens was determined by cuttingsamples with a cryotome and taking images with SEM(Hitachi S-3400N, Tokyo, Japan). Images were analyzedwith image analysis software (AxioVision, Carl Zeiss, Jena,
42 Page 2 of 11 Journal of Materials Science: Materials in Medicine (2019) 30:42
Germany) and average thickness was calculated at about246 ± 49 μm.
An algorithm was developed using Scilab software(Version 5.4.1, ESI Group, Rungis, France) to compute thedata of the static testing and calculate ultimate tensile stressand elongation at break automatically .
2.5 Dynamic light scattering (DLS) and zeta-potential
Particle size was measured with a Zetasizer Nano ZS fromMalvern Instruments (Malvern, UK). Size measurementswere carried out in disposable sizing cuvettes (DTS0012) at20 °C. For data analysis Malvern Zetasizer Software Ver-sion 7.03 was used.
2.6 Differential scanning calorimetry (DSC)
Differential scanning calorimetry (DSC) measurementswere carried out on a Netzsch DSC204 Phoenix connectedto Netzsch TASC 414/3A controller equipped with CC-200 cooling controller from Netzsch (Selb, Germany).PCL scaffolds were sealed in alumina pans with piercedlid and exposed to a double heating cycle: Samples wereheated up from room temperature to 120 °C with a heatingrate of 10 °C/min. Subsequently, samples were cooleddown to −100 °C with a cooling rate of 10 °C/min andheated up again to 120 °C with a heating rate of 10 °C/min. Proteus thermal analysis software (Netzsch) wasused to quantify melting temperature as peak temperature(Tm), enthalpy of fusion (HF), glass transition temperature(Tg) and change in heat capacity at glass transition (Δcp).Both heating cycles were evaluated. For quality controlreasons, another set of thermograms was recorded on aTA Q2000 by TA instruments (New Castle, USA).Heating cycles and sample preparation are identical to theones performed on Netzsch DSC. Universal Analysissoftware (TA Instruments) was used to quantify meltingtemperature (Tm), enthalpy of fusion (HF), glass transitiontemperature (Tg) and change in heat capacity at glasstransition (Δcp). Data was merged by averaging for a
comprehensive overall median value, since all measuredsets were identical.
2.7 Size exclusion chromatography (SEC)
SEC measurements were carried out on a set of PSS GRAMcolumns (precolumn, 5 μm, 2 × 1000 Å, 5 μm) (Mainz,Germany) with THF as eluent at 40 °C with a flow rate of1 mL/min. Injection volume was 100 μL with a sampleconcentration of 2 mg/mL. Chromatograms were recordedwith a refractive index detector Agilent 1260 Infinity fromAgilent (Santa Clara, USA) at 35 °C and a viscosity detectorPSS DVD1260 from PSS (Mainz, Germany) at 30 °C whichallowed using an universal calibration. WinGPC Unichromsoftware (PSS) was used to process the chromatograms.
Electrospun PCL fiber mats were sterilized using electronbeam (β), gamma radiation (γ) and X-rays (X-ray) at dosesof 25 and 33 kGy each. It has been reported that γ-radiationdamages PCL and changes both its mechanical and che-mical properties [14, 24]. Since the methods used here,namely electron beam and X-rays sterilization differ in theirphoton energy [11, 26], they might have less impact on thematerial properties of electrospun PCL fiber mats. Changesregarding mechanical and thermal properties were mon-itored. Preliminary studies, even though not comprehen-sively performed, proved that sterilization itself did notnegatively affect biocompatibility of the scaffolds as shownin literature .
3.1 Scaffold properties
Fiber mats were produced with different collector speeds, inorder to control the alignment of the fibers. The mats wereinvestigated regarding the fiber orientation by scanningelectron microscopy (SEM) (see Fig. 1). Fiber mats pro-duced with a higher collector speed showed alignment,while fiber mats produced with a low collector speed were
Figure 1 SEM micrographs ofan aligned (left) and non-aligned(right) PCL fiber mat
Journal of Materials Science: Materials in Medicine (2019) 30:42 Page 3 of 11 42
non-aligned (see Supplementary Information Figs 10 and11). The fiber diameter of the aligned (a) PCL fiber matswas 2.1 ± 0.6 μm and for the non-aligned (random, r) 2.2 ±0.5 μm. Furthermore, SEM images proved that fiber matswere of consistent quality and showed a homogenous fibermorphology distribution.
3.2 Mechanical properties
PCL scaffolds were tested to determine ultimate tensilestrength and elongation at break. For the control set, eachkind of irradiation, and both doses at least ten specimenswere tested following the protocol developed by Zernetsch. Data were computed with a self-developed SciLabalgorithm and plotted as boxplots for non-aligned andaligned PCL scaffolds separately (see Fig. 2). The boxes forboth types of untreated fiber mats showed a high width,which implied a great spread of the data. Median of ultimatetensile strength was 6 N/mm² and 5 N/mm² for the non-aligned and aligned scaffolds, respectively. After irradia-tion, the ultimate tensile strength of non-aligned PCLscaffolds decreased for all irradiation types and intensitiescompared to control group to about 2/3 of the control value.Such a decrease in the mechanical strength has beenobserved by Bosworth et al. as well . The median valueswere in range of 2.4–3.3 N/mm². The effects seemed not tobe dependent on dose or type of irradiation. For the alignedfiber mats, however, the median values for ultimate tensilestrength varied between 5.5 and 7.5 N/mm² and thereforeremained more or less unchanged after sterilization.
The elongation at break (see Fig. 3) was 775% for non-aligned and 750% for aligned PCL fiber mats before ster-ilization. For the non-aligned samples, no effect of the
sterilization was observed. However, for aligned samples, aslight increase in elongation at break was measured afterirradiation from 750% for control to ~900% for irradiatedsamples. Again, no significant effects of the dose or type ofirradiation on the mechanical properties were observed.
3.3 Size exclusion chromatography (SEC)
PCL of sterilized fiber mats was checked for changes inmolecular weight after sterilization. Chromatograms wererecorded on a THF-SEC using refractive index and visc-osity detector allowing for universal calibration. Eachsample was tested at least three times (n ≥ 3). Numericalaverage and standard deviation were calculated and twosample t-tests were performed to check for significantdifferences by using degrees of freedom and determiningthe corresponding p-values (* ≤ 5%, ** ≤ 1%, *** ≤ 0.1%,n.s.= not significant).
Figure 4 shows two exemplary SEC chromatograms andtheir refractive index detectors signals. In both cases, onlyone signal with a polydisperse molecular weight distributionwas observed. According to manufacturer, the PCL used forthe fiber mat production had a molecular weight of 80,000–120,000 g/mol. This was verified by our SEC measure-ments, which showed that unsterilized but processed PCLhad an average molecular weight M̅n of 95,000 g/mol. ThePCL from fiber mats sterilized with gamma radiation at adose of 33 kGy showed a significant higher retention timecompared to PCL from a non-sterilized sample corre-sponding to lower a M̅n of 67,500 g/mol.
Such a reduction in molecular weight was established forall PCL samples from sterilized fiber mats (see Fig. 5). The
Figure 2 Tensile stress (n ≥ 10) for electrospun PCL scaffolds. Shownare control samples for aligned (a) and non-aligned (r) fibers andsterilized samples. Use of gamma (γ), X-ray (x) and beta (ß) radiationat 25 and 33 kGy. Doted lines display the median values for controlsets of aligned (red) and non-aligned (blue) samples
Figure 3 Elongation at break (n ≥ 10) for electrospun PCL scaffolds.Shown are control samples for aligned (a) and non-aligned (r) fibersand sterilized samples. Use of gamma (γ), X-ray (x) and beta (ß)radiation at 25 and 33 kGy. Doted lines display the median values forcontrol sets of aligned (red) and non-aligned (blue) samples
42 Page 4 of 11 Journal of Materials Science: Materials in Medicine (2019) 30:42
higher the irradiation dose the more chain cleavage tookplace and the lower the average molecular weight.
3.4 Thermal properties and crystallinity
Sterilized fiber mats were analyzed using differential scan-ning calorimetry (DSC) techniques on two different DSCsetups with three identical runs each to verify the results.Exemplary thermograms are shown in Fig. 6. It can be seenthat thermograms resulting from the 1st and 2nd heatingcycle differed slightly, which was due to the differentthermal history of the material. While the sample in the firstheating cycle was material that crystallized in the electro-spinning process by fast evaporation of a solvent, thesample in the second heating cycle crystallized during acontrolled cooling process. Thus, only the first heating cycleallowed to draw conclusions about the actual crystallinity offiber mats, while the second heating cycle probes the abilityto crystallize. Furthermore, for the first heating cycle afibrous material is used, which might have limited thermalcontact with the aluminum pan and therefore can causeartefacts. Unless otherwise noticed, all data and conclusionsin the following chapter are drawn from the 2nd DSCheating cycle and therefore depict the materials generalcapability to crystallize.
Figure 6 depicts the differences between 1st and 2ndheating cycle. In both cases, a clearly defined peak wasvisible. However, for the second heating cycle the meltingstarted earlier and the melting peak was broader. Further-more, the melting point measured as peak temperature wassomewhat lower.
Comparing thermograms of a sterilized sample (μ-irra-diation, 33 kGy) and non-irradiated but processed PCL as acontrol (see Fig. 7), differences in height of melting peak
and, therefore, probably a difference in enthalpy of fusionwas observed. Since all measurements looked similar andshowed peaks in the same regions, data were processed withan automated procedure to compare them. Thermogramswere evaluated regarding melting point Tm, enthalpy offusion ΔHF, glass transition temperature Tg and the changein heat capacity Δcp. T-testing was performed to check forsignificance of changes against control group and betweenirradiation types and doses.
The aligned fibers had a higher melting temperaturecompared to randomly oriented fibers. Sterilization led to anincrease in average melting temperature of about 1–2 °C at adose of 33 kGy.
Besides melting temperature, also glass transition tem-peratures were evaluated. In some cases, a lower Tg wasobserved for PCL from sterilized samples (see Fig. 8
Figure 4 THF-SEC chromatogram for PCL (red) and PCL, sterilizedwith gamma irradiation at a dose of 33 kGy (black)
Figure 5 (top) molecular weights (M̅n) of sterilized scaffolds deter-mined by THF-SEC for sterilized PCL fiber mats (n ≥ 3, SD). (bottom)polydispersity of sterilized PCL scaffolds determined by THF-SEC(n ≥ 3). Shown are control samples for aligned (a) and non-aligned (r)fibers and sterilized samples. Use of gamma (γ), X-ray (x) and beta (ß)radiation at 25 and 33 kGy. Statistics was performed using two samplet-test (* ≤ 5%, ** ≤ 1%, *** ≤ 0.1%, n.s.= not significant)
Journal of Materials Science: Materials in Medicine (2019) 30:42 Page 5 of 11 42
(bottom)). However, changes are small and in most casesstatistically not significant. No clear trend was observed forsamples irradiated with different doses. In addition, the typeof radiation did not influence Tg in a consistent manner.
Change in heat capacity (Δcp) was evaluated since it isindicating the fraction of amorphous material. It wasobserved that Δcp was lowered significantly after irradiationtreatment. This effect was dependent on dose and type ofirradiation. Δcp was lowered from 0.25 J/g*K for non-aligned unsterilized samples to a minimum of 0.17 J/g*Kfor X-radiation and a dose of 33 kGy.
Degree crystallization (Xc) can be estimated from theratio of measured ΔHF Tmð Þ (see Supplementary Informa-tion Fig. 14) and the enthalpy of fusion of a completely
crystalline material ΔH0FðT0mÞ:
Xc ¼ ΔHFðTmÞΔH0FðT0mÞð1Þ
Enthalpy of fusion of completely crystalline PCL ΔH0F T0m� �
has been reported as 139.3 J*g−1 . With these data, thedegree of crystallinity was calculated for all samples anddepicted in Fig. 9. Again, it was observed that aligned fiberswere more crystalline than randomly oriented fibers,although the second heating cycle was evaluated.
Furthermore, it was observed that all types and doses ofirradiation used for sterilization led to a significant increasein crystallinity, as it was already expected after evaluationof Δcp (see above). This effect was significantly stronger forirradiation with electrons and X-rays compared to
Figure 6 exemplary DSC thermogram of PCL sample sterilized withgamma irradiation at dose of 33 kGy. Shown are the 1st (dotted line),2nd heating cycle (solid line) and relevant measurement points forsample evaluation
Figure 7 DSC thermogram showing differences between a sterilized(γ-radiation, 33 kGy) PCL sample (solid line) and an unsterilized PCLsample acting as control group (dotted line)
Figure 8 (top) Tm for sterilized PCL fiber mats. (bottom) Tg for ster-ilized PCL fiber mats (n ≥ 6, SD). Shown are control samples foraligned (a), non-aligned (r) fibers and sterilized samples. Use ofgamma (y), X-ray (x) and beta (ß) radiation at 25 and 33 kGy. Sta-tistics (n= 6) was performed using two sample t-test (* ≤ 5%, ** ≤ 1%,*** ≤ 0.1%, n.s.= not significant)
42 Page 6 of 11 Journal of Materials Science: Materials in Medicine (2019) 30:42
y-irradiation. The increase in crystallinity amounted to up to9.9% for X-ray- and β-irradiation at 33 kGy.
Aligned and non-aligned PCL scaffolds were produced andevaluated. Fiber alignment was evaluated by SEM imaging,as shown in Fig. 1. It was shown that homogenous fibers ofaligned and non-aligned nature (see Supplementary Infor-mation Figs 11 and 12) were produced. It is known that thisorientation of fibers comes along with various changes inthe material properties such as mechanical properties, fiberdiameter and crystallinity . Furthermore fiber diameterwas analyzed and showed slightly thinner fibers for alignedsamples. This slight difference in fiber diameter might alsoinfluence the thermal properties and crystallinity after ster-ilization, however, the main influence of the fiber orienta-tion is on mechanical properties.
PCL scaffolds were tested to determine ultimate tensilestrength and elongation at break. ISO 13934 is a commonlyused standard to determine tensile properties of fabrics,however for electrospun fiber structures a reliable standardfor mechanical characterization does not exist . Incon-sistent testing of electrospun structures throughout theavailable literature creates obstacles for the comparison withresults from other research groups and highlights thenecessity for a uniform testing method. Therefore, Zer-netsch developed a protocol for testing electrospun fibermats and analyzing data, based on the norm ISO 527 formechanical testing of plastics .
Augustine et al.  and Bosworth et al.  tested theinfluence of γ-sterilization on electrospun PCL scaffolds.Both groups worked with a replicate of 5 specimens. Usinga static setup, Augustine et al.  produced highly dis-ordered fiber mats, while Bosworth et al.  used arotating drum with a circumferential speed of 3.77 m/s,which is significantly lower than the speed used here(8 m/s). In addition, electrospinning solutions and otherprocess parameters were significantly different, as well astesting parameters.
Both groups found no significant difference of elonga-tion at break before and after γ-irradiation treatment nor aninfluence of irradiation dose on the same. However,Augustine et al.  found that ultimate tensile stress ofaligned scaffolds first increased with irradiation treatmentcompared to a non-sterilized control while decreasing athigher irradiation doses. Bosworth et al.  on the otherhand showed that ultimate tensile stress decreased whennon-aligned scaffolds were exposed to irradiation while thedose showed no significant effect on ultimate tensile stress.
We observed that for non-aligned scaffolds upon ster-ilization the ultimate tensile strength decreased slightly (seeFig. 2), while elongation at break remained unchanged (seeFig. 3). On the other hand, for aligned scaffolds the ultimatetensile strength did not change significantly, while theelongation at break showed a trend for slightly highermedian values, but with a large spreading of the data. Thus,in particular for the aligned fiber mats the results obtainedwere not completely in line with the findings of Augustineet al. and Bosworth et al. However, this was probably due toinconsistent electrospinning and tensile testing protocols.
High energy radiation does not only sterilize a medicaldevice made from polymers, however, it can also result in ascission of the polymer chains . Formation of radicals inthe polymer matrix, due to chain scission, might also resultin crosslinking or branching of polymer chains. Thus, SECmeasurements were performed. These indicated a lowermolecular weight (M̅n) after sterilization due to irradiationinduced chain scission, as shown in Fig. 5. This was furthersubstantiated by a change in polydispersity of the PCL fromirradiated samples. We used t-testing to check for differ-ences between aligned and non-aligned samples resultingfrom fiber diameter and alignment. In addition, irradiationtypes and different irradiation doses were tested for sig-nificant differences against each other and against non-sterilized control. As depicted in Fig. 5, polydispersityincreased significantly after sterilization by high-energyirradiation, which was another indication for polymer chainscission [31, 32]. The loss in molecular weight is in linewith the observations of Bosworth et al. . Furthermore,an influence of the type of sterilization was observed. Oncemore, the different irradiation doses and types were testedagainst each other and against a non-sterilized control to
Figure 9 crystallinity of sterilized PCL samples (n ≥ 6, SD). Shown arecontrol samples for aligned (a) and non-aligned (r) fibers and sterilizedsamples. Use of gamma (y), X-ray (x) and beta (ß) radiation at 25 and33 kGy. Statistics (n= 6) was performed using two sample t-test (* ≤5%, ** ≤ 1%, *** ≤ 0.1%, n.s.= not significant)
Journal of Materials Science: Materials in Medicine (2019) 30:42 Page 7 of 11 42
check for significant differences. γ-Irradiation with 33 kGyhad the strongest impact and led to a significant molecularweight reduction (M̅n) of 30 ± 1%. The M̅w (see Supple-mentary Information Fig. 13) decreased slightly as well. Ingeneral, γ-irradiation should have the highest capability tocleave the polymer chains because of its higher photonenergy compared to β- and X-ray irradiation [11, 26].However, also β- and X-ray irradiation resulted in chainscission and a reduction of M̅n to 69,100 g/mol for β-radiation and 68,400 g/mol for X-ray for 33 kGy irradiationdose and aligned fiber mats, indicating that also here photonenergy is high enough for some chain scission. However,the reduction in M̅n is statistically significant less pro-nounced for β- and X-ray irradiation compared to the γ-irradiation. Therefore, these methods appeared more sui-table for sterilization of medical products produced fromPCL.
Irradiation and chain scission as primary reaction createsradicals, which in a secondary reaction can lead to cross-linking. However, SEC chromatograms showed no indica-tion for crosslinking products, like a high molecular weightshoulder in the distribution. This could be because thesolutions were filtered before SEC-analysis, which shouldremove any microgel particles. Therefore, DLS measure-ments were performed with non-filtered polymer solutions.This technique should be able to detect such microgelseasily. However, no such particles were found, whichconcluded the presumption that no crosslinking occurred.
The significant reductions in average molecular weightwere expected to result in a decrease in mechanical prop-erties, which was not observed (see above). However, thereduced polymer chain length was presumed to be com-pensated in particular in the aligned fiber mats. The strengthof a material strongly depends on the degree of crystallinity;therefore, thermal properties and crystallinity of the sampleswere investigated.
Thermal properties and crystallinity of materials fabri-cated for medical applications can be critical for their per-formance , especially due to relatively low melting pointof PCL of 60 °C . Considerable lowering of this meltingpoint could lead to failure of the implant since human bodytemperature can reach up to 42 °C . Hence sterilizationmethod and dose should be chosen according to the lowestimpact on the original material properties. As shown in Fig.6, differences between 1st and 2nd heat cycle can bemeasured. These differences were attributed to a differentsize distribution of crystalline regions caused by differentthermal history of the samples. Thermograms were eval-uated regarding melting point Tm, enthalpy of fusion ΔHF,glass transition temperature Tg and the change in heatcapacity Δcp. T-testing was performed to check for sig-nificance of changes against control group and betweenirradiation types and doses.
Aligned fibers showed a higher Tm compared to non-aligned ones, which might be due to increased crystallinityresulting from stretching of fibers in electrospinning processand associated improved orientation of polymer chains .However, taking into account the changes were only sig-nificant for a few comparisons it can be concluded that allsterilization doses and techniques had no big impact onmelting peak temperature of the materials (see Fig. 8 (top)).Tg was also not affected in a statistically significant andconsistent manner (see Fig. 8 (bottom)).
Change in heat capacity (Δcp) at glass transition is ameasure for fraction of amorphous material in the sample. Asmall change in Δcp indicates a low amorphous and there-fore a high crystalline portion. Δcp was lower for PCL fromaligned fiber mats, indicating a smaller portion of amor-phous material (see Fig. 10). This behavior was unexpectedfor PCL-samples, which have been processed in the sameway except for some stretching of the fibers. In the secondheating cycle thermal or mechanical history of the sampleshould have been eradicated. However, it has been shownthat a memory effect regarding crystallinity, mainly due toremaining small crystallites, can be observed for polymerseven after melting [35–37]. Therefore, even after meltingthe polymer once, a lower Δcp for aligned samples asconsequence of the stretching during electrospinning can beobserved (see Fig. 5, top). Upon sterilization, Δcp wasreduced significantly, thus the fraction of amorphousmaterial is reduced by the sterilizations methods used here.While type of irradiation used did not make very much of adifference, used dose had a strong influence. The higher thedose the lower Δcp. T-testing showed that decrease in Δcp issignificant after sterilization for all tested irradiation types
Figure 10 Change in heat capacity (Δcp) for sterilized PCL fiber mats(n ≥ 6, SD). Shown are control samples for aligned (a) and non-aligned(r) fibers and sterilized samples. Use of gamma (y), X-ray (x) and beta(ß) radiation at 25 and 33 kGy. Statistics (n= 6) was performed usingtwo sample t-test (* ≤ 5%, ** ≤ 1%, *** ≤ 0.1%, n.s.= not significant)
42 Page 8 of 11 Journal of Materials Science: Materials in Medicine (2019) 30:42
and doses. In conclusion, the evaluation of change in heatcapacity at the glass transition indicated that used ster-ilization methods increased the degree of crystallinity.However, Δcp is an indirect measure for degree of crystal-linity and, therefore, heat of fusion ΔHF (see SupplementaryInformation Fig. 14), the area of the melting peak, wasevaluated as well.
ΔHF is, beside X-ray investigations, probably the mostdirect access to degree of crystallinity. Samples with a highdegree of crystallinity show a high ΔHF, since crystallineregions need energy to break up their order and relatedintermolecular interactions. It was observed that melting ofthe polymers for a relatively short time did not eradicateordering of the polymer chains completely. Although thepolymer chains became mobile, the viscosity of melt wasstill very high and restructuring of the polymer chain con-formation would have required a long time. The polymerhowever was cooled down before chain ordering due to theelectrospinning process was completely eradicated (memoryeffect) [35–37]. A significant increase in crystallinity wasobserved after irradiation. This effect was once moredependent on dose or type of irradiation used (see Fig. 9).Irradiation seemed to affect and cleave the polymer chains,which should subsequently rearrange resulting in regions ofhigher crystallinity and therefore an overall smaller amor-phous fraction. Since these effects were stronger at higherirradiation doses, a low dose should be chosen for medicaldevices sterilization.
Taken together, it can be clearly observed that steriliza-tion by gamma (γ), X-ray (x) and beta (ß) radiation at 25and 33 kGy led to changes regarding PCL’s thermal prop-erties and crystallinity. There was a significant influence ofirradiation type used for sterilization on change in heatcapacity (Δcp) as well as on enthalpy of fusion (ΔHF). Thedecrease in Δcp and simultaneous increase in ΔHF withirradiation, which are both statistically significant, indicatedincreasing crystallinity after sterilization. This wasexplained to be a consequence of chain scission andtherefore reduced average molecular weight, which wasestablished by SEC measurements. The shorter polymerchains can crystallize more easily resulting in higher degreeof crystallinity. While on the one hand decreased molecularweight should also result in reduced mechanical strength, onthe other hand a higher crystallinity should improvemechanical strength. Hence, maintained mechanical prop-erties were a consequence of higher crystallinity compen-sating effects from polymer chain scission. Changes in Tmand Tg upon sterilization were minor and not consistentlysignificant. It was observed that a higher irradiation doseduring the sterilization process went along with a higherimpact on the PCL scaffolds. Therefore, a low irradiationdose should be favorable to minimize changes in thermalproperties and crystallinity of PCL.
It was shown that all three sterilization techniques had animpact on electrospun PCL scaffolds. Since none of thesterilization methods led to a failure of the fiber mats, all ofthem were proven to be generally applicable for sterilizationof PCL fiber mats. However, use of β-irradiation seemspreferable since it has less effect on the scaffolds comparedto γ-irradiation. Furthermore medical device sterilization byβ-radiation is easily accessible, cheap and more data areavailable for the method compared to sterilization by X-rays.
4.1 Conclusion and outlook
Sterilization of medical devices is inevitable to avoid postoperation infections. However, sterilization methods have tobe reliable and chosen according to the used materials prop-erties. The impact of three different sterilization techniques (β,γ and X-ray) on electrospun PCL scaffolds was evaluated. Itwas shown that material properties of PCL in electrospunfiber mats were affected by all three sterilization techniques.
The irradiation led to a polymer chain scission and adecreased average molecular weight M̅n. The effect wasmore pronounced for higher irradiation doses. γ-irradia-tion with dose 33 kGy led to a decrease in M̅n of around30%. Polymer crosslinking as consequence of irradiationinduced chain scission was ruled out since no indicationsfor microgel particles were found in SEC and DLS mea-surements. Thermal properties and crystallinity of PCLwere affected as well. While melting temperature andglass transition temperature were almost unchanged,change in heat capacity (Δcp) and enthalpy of fusion(ΔHF) were effected significantly. The changes indicatedan improved crystallization process for sterilized samples.For mats with aligned fibers, ultimate tensile strength andelongation at break were even slightly increased whilethey remained unchanged for mats with non-alignedfibers. This slight improvement in mechanical propertiesof aligned scaffolds despite decreased polymer chainlength was ascribed to the increase in crystallinity. Thescission of long polymer chains into smaller ones led to anincreased ability to form regions with a higher crystal-linity and therefore higher mechanical strength, whichovercomes negative effects of polymer chain scission.Electron beam had less effect on PCL than y-irradiation.Furthermore, it has been established already as a ster-ilization method. Therefore, electron beam sterilization isrecommended for PCL fiber mats.
Acknowledgements This research project has been supported by theDFG FOR 2180 “Gradierte Implantate für Sehnen-Knochen-Verbin-dungen“. Furthermore the authors would like to thank “Thünen-Institutfür Agrartechnologie” for assistance in performing DSC measure-ments. The authors would like to thank Michael Bode and AlexanderBecker (Institute for Multiphase Processes, Gottfried Wilhelm LeibnizUniversität Hannover, Hannover, Germany) for discussions.
Journal of Materials Science: Materials in Medicine (2019) 30:42 Page 9 of 11 42
Compliance with ethical standards
Conflict of interest The authors declare that they have no conflict ofinterest.
Publisher’s note: Springer Nature remains neutral with regard tojurisdictional claims in published maps and institutional affiliations.
1. Lerouge S, Simmons A. Sterilisation of biomaterials and medicaldevices. Woodhead Publishing series in biomaterials, no. 46.Philadelphia, PA: Woodhead Pub; 2012.
2. dos Santos V, Brandalise RN, Savaris M. Engineering of bio-materials. Cham: SpringerLink: Bücher. Springer; 2017.
3. Mendes GCC, Brandão TRS, Silva CLM. Ethylene oxide ster-ilization of medical devices: a review. Am J Infect Control.2007;35:574–81. https://doi.org/10.1016/j.ajic.2006.10.014.
4. Hee Lee M, Joo Park B, Chang Jin S, Kim D, Han I, Park J-C.et al. Removal and sterilization of biofilms and planktonic bacteriaby microwave-induced argon plasma at atmospheric pressure. NewJ Phys. 2009;11:115022. https://doi.org/10.1088/1367-2630/11/11/115022..
5. Benson RS. Use of radiation in biomaterials science. Nucl InstrumMethods Phys Res Sect B: Beam Interact Mater At. 2002;191:752–7. https://doi.org/10.1016/S0168-583X(02)00647-X.
6. Noah EM, Chen J, Jiao X, Heschel I, Pallua N. Impact of ster-ilization on the porous design and cell behavior in collagen spongesprepared for tissue engineering. Biomaterials. 2002;23:2855–61.https://doi.org/10.1016/S0142-9612(01)00412-4.
7. Govindaraj S. Systematic Review on Sterilization Methods ofImplants and Medical Devices. Implants and Medical Devices. IntJ ChemTech Res. 2015;8:897–911.
8. Hutmacher D, Hürzeler MB, Schliephake H. A review of materialproperties of biodegradable and bioresorbable polymers anddevices for GTR and GBR applications. Int J Oral MaxillofacImplants. 1996;11:667–78.
9. Collier JP, Sperling DK, Currier JH, Sutula LC, Mayor MB.Impact of gamma sterilization on clinical performance of poly-ethylene in the knee. J Arthroplast. 1996;11:377–89. https://doi.org/10.1016/S0883-5403(96)80026-X.
10. Athanasiou K. Sterilization, toxicity, biocompatibility and clinicalapplications of polylactic acid/ polyglycolic acid copolymers.Biomaterials. 1996;17:93–102. https://doi.org/10.1016/0142-9612(96)85754-1.
11. Dai Z, Ronholm J, Tian Y, Sethi B, Cao X. Sterilization techniquesfor biodegradable scaffolds in tissue engineering applications. J TissueEng. 2016;7:2041731416648810. https://doi.org/10.1177/2041731416648810.
12. Hutmacher DW. Scaffolds in tissue engineering bone and carti-lage. Biomaterials. 2000;21:2529–43.
13. Woodruff MA, Hutmacher DW. The return of a forgotten polymer—Polycaprolactone in the 21st century. Prog Polym Sci. 2010;35:1217–56. https://doi.org/10.1016/j.progpolymsci.2010.04.002.
14. Bosworth LA, Gibb A, Downes S. Gamma irradiation of elec-trospun poly(ε-caprolactone) fibers affects material properties butnot cell response. J Polym Sci B Polym Phys. 2012;50:870–6.https://doi.org/10.1002/polb.23072.
15. Zahedi P, Rezaeian I, Ranaei-Siadat S-O, Jafari S-H, Supaphol P.A review on wound dressings with an emphasis on electrospunnanofibrous polymeric bandages. Polym. Adv. Technol. 2009;35.https://doi.org/10.1002/pat.1625
16. Lee B-K, Ju YM, Cho J-G, Jackson JD, Lee SJ, Yoo JJ. et al. End-to-side neurorrhaphy using an electrospun PCL/collagen nerveconduit for complex peripheral motor nerve regeneration. Bio-materials. 2012;33:9027–36. https://doi.org/10.1016/j.biomaterials.2012.09.008.
17. Hasan A, Memic A, Annabi N, Hossain M, Paul A, Kha-demhosseini A. et al. Electrospun scaffolds for tissue engineeringof vascular grafts. Acta Biomater. 2014;10:11–25. https://doi.org/10.1016/j.actbio.2013.08.022.
18. Xue J, He M, Liu H, Niu Y, Crawford A, Zhang L. et al. Drugloaded homogeneous electrospun PCL/gelatin hybrid nanofiberstructures for anti-infective tissue regeneration membranes. Bio-materials. 2014;35:9395–405. https://doi.org/10.1016/j.biomaterials.2014.07.060.
19. Font Tellado S, Balmayor ER, van Griensven M. Strategies toengineer tendon/ligament-to-bone interface: Biomaterials, cellsand growth factors. Adv Drug Deliv Rev. 2015;94:126–40.https://doi.org/10.1016/j.addr.2015.03.004.
20. Rainer A, Centola M, Spadaccio C, Gherardi G, Genovese JA,Trombetta M. et al. Comparative study of different techniques forthe sterilization of poly-L-lactide electrospun microfibers: effec-tiveness vs. material degradation. Int J Artif Organs. 2010;33:76–85.
21. Bhaskar P, Bosworth LA, Wong R, O'brien MA, Kriel H, Cart-mell SH. et al. Cell response to sterilized electrospun poly(ɛ-caprolactone) scaffolds to aid tendon regeneration in vivo. JBiomed Mater Res A. 2017;105:389–97. https://doi.org/10.1002/jbm.a.35911.
22. Kudoh H, Sasuga T, Seguchi T. High-energy ion irradiationeffects on polymer materials. In: Clough RL, Shalaby SW, (eds.).Irradiation of Polymers. Vol. 620. Washington, DC: AmericanChemical Society; 1996. p. 2–10.
23. Otaguro H, de Lima L, Parra DF, Lugao A. High-energy radiationforming chain scission and branching in polypropylene. RadiatPhys Chem. 2010;79:318–24. https://doi.org/10.1016/j.radphyschem.2009.11.003.
24. Augustine R, Saha A, Jayachandran VP, Thomas S, Kalarikkal N.Dose-dependent effects of gamma irradiation on the materialsproperties and cell proliferation of electrospun polycaprolactonetissue engineering scaffolds. international. J Polym Mater PolymBiomater. 2015;64:526–33. https://doi.org/10.1080/00914037.2014.977900.
25. Zernetsch H, Repanas A, Rittinghaus T, Mueller M, Alfred I,Glasmacher B. Electrospinning and mechanical properties ofpolymeric fibers using a novel gap-spinning collector. FibersPolym. 2016;17:1025–32. https://doi.org/10.1007/s12221-016-6256-7.
26. Cottam E, Hukins DWL, Lee K. et al. Effect of sterilisation bygamma irradiation on the ability of polycaprolactone (PCL) to actas a scaffold material. Med Eng Phys. 2009;31:221–6. https://doi.org/10.1016/j.medengphy.2008.07.005.
27. Zernetsch H. Gezielte Beeinflussung der Mikro- und Makros-truktur polymerer Trägerstrukturen beim Elektrospinnen. Berichteaus dem IMP, Band 1. Garbsen: PZH Verlag; 2016.
28. Tiwari A, Raj B. Reactions and mechanisms in thermal analysis ofadvanced materials. Hoboken, New Jersey, Salem, Massachusetts:John Wiley & Sons; Scrivener Publishing; 2015.
29. Cipitria A, Skelton A, Dargaville TR. et al. Design, fabricationand characterization of PCL electrospun scaffolds—a review. JMater Chem. 2011;21:9419. https://doi.org/10.1039/c0jm04502k.
30. Kancheva M, Toncheva A, Manolova N. et al. Enhancing themechanical properties of electrospun polyester mats by heattreatment. Express Polym Lett. 2015;9:49–65. https://doi.org/10.3144/expresspolymlett.2015.6.
42 Page 10 of 11 Journal of Materials Science: Materials in Medicine (2019) 30:42
31. Luo Y, Li P, Jiang B. The estimation of the polydispersity indexof molecular weight distribution with a radiation crosslinkingtechnique: I. The effect of molecular weight distribution on theradiation crosslinking of polyethylene. Int J Radiat Appl InstrumC Radiat Phys Chem. 1987;29:415–8. https://doi.org/10.1016/1359-0197(87)90016-6.
32. O’Donnell JH, Rahman NP, Smith CA. et al. Chain scission andcross-linking in the radiation degradation of polymers: limitationson the utilization of theoretical expressions and experimentalresults in the pregel region. Macromolecules. 1979;12:113–9.https://doi.org/10.1021/ma60067a024.
33. Speranza V, Sorrentino A, de Santis F. et al. Characterization ofthe polycaprolactone melt crystallization: Complementary opticalmicroscopy, DSC, and AFM studies. TheScientificWorldJournal.2014;2014:720157. https://doi.org/10.1155/2014/720157.
34. Harrison TR, Longo DL, Kasper DL. et al. Harrison’s principlesof internal medicine. In: Dan L. Longo et al. Editors, 18th edn.New York: McGraw-Hill; 2012.
35. Martins JA, Zhang W, Brito AM. Origin of the melt memoryeffect in polymer crystallization. Polymer. 2010;51:4185–94.https://doi.org/10.1016/j.polymer.2010.07.010.
36. Chen X, Mamun A, Alamo RG. Effect of level of crystallinity onmelt memory above the equilibrium melting temperature in arandom ethylene 1-butene copolymer. Macromol Chem Phys.2015;216:1220–6. https://doi.org/10.1002/macp.201500068.
37. Muthukumar M. Communication: Theory of melt-memory inpolymer crystallization. J Chem Phys. 2016;145:31105. https://doi.org/10.1063/1.4959583.
Journal of Materials Science: Materials in Medicine (2019) 30:42 Page 11 of 11 42
Impact of sterilization by electron beam, gamma radiation and X-rays on electrospun poly-(ε-caprolactone) fiber matsAbstractIntroductionMaterials and methodsElectrospinning of PCLSterilizationScaffold morphologiesMechanical characterizationDynamic light scattering (DLS) and zeta-potentialDifferential scanning calorimetry (DSC)Size exclusion chromatography (SEC)
ResultsScaffold propertiesMechanical propertiesSize exclusion chromatography (SEC)Thermal properties and crystallinity
DiscussionConclusion and outlook
ACKNOWLEDGMENTSCompliance with ethical standards